Date post:  27Apr2015 
Category: 
Documents 
Author:  choidoyoung 
View:  8,070 times 
Download:  2 times 
Chapter 13. Solid  Liquid Separation13. INTRODUCTION The process of grinding and classification involves the use of large quantities of water. In the gold industry for instance, the rule of thumb is a tonne of water for a tonne of ore. This bulk of water has to be separated or reduced for down stream treatment for recovery of the mineral in the ore. The separation of solids from liquids is usually achieved by gravity sedimentation in thickeners. For fine particles this is a slow process. In general 7580 % of the water can be separated and removed by thickeners. For further water removal, filters are used where in excess of 90% of the water can be removed. The thickener operation can be a batch or continuous process, with either cocurrent or countercurrent flow of underflow and overflow slurries. The filtering operation may also be batch or continuous. For rapid solidliquid separations, centrifugal forces are used and equipment similar to those described under classification are employed, ha this chapter, we shall deal mostly with thickeners working under gravitational forces. 13.1. Design Features of Thickeners Thickeners are essentially clarifiers producing a clearer over flow. The design considerations are based on the settling rates of the slowest settling particles and conditions for minimum disturbance of the medium (water) through which the solid particles are allowed to settle. To achieve these objectives cylindrical tanks with conical or flat bottoms are used and the velocity of the feed slurry entering the settling tank is minimised to reduce turbulence in the settling tank. A schematic diagram of a typical thickener is shown in Fig. 13.1. The feed in the form of slurry is generally guided by a launder, which is laid at a slope just sufficient for the slurry to flow without depositing any solids. The feed launder terminates in a feed well located at the centre of the tank. The feed well is designed to break the fall of the slurry and dissipate the energy. The feed well is concentric with the rake driving shaft. The rakes are bolted or welded on to this drive shaft and for long and large rakes they have additional support from cables. Usually four rakes are employed of which two may be short and two long. Attached to the rakes and below them are spikes, particularly in situations where the sludge is thick. The spikes help to break up the sludge and render it more suitable for pumping. The rakes are driven by a motor which is mounted on a plate above the well. An alternative is to mount the drive motor on a track running along the rim of the tank. A bridge usually runs from the periphery to the centre of the tank. It is supported by the wall of the feed well and the rim of the tank. The bridge serves as a walkway and also carries an open launder (or pipe), which carries the slurry to the feed well. In some designs the bridge spans the entire length of the tank. As in clarifiers, the bottom of most tanks slope towards the centre where the thickened underflow sludge accumulates. When a flat bottomed tank is designed, the settled sludge builds up to form its own slope depending on the angle of repose of the material thus forming an artificial sloping tank bottom. The sludge collected at the bottom is discharged through an outlet shaped like a cone with steep cone angle. Alternately, the thickened slurry is swept
402
towards a trench at the bottom of the tank. Usually a scraper is installed for smooth delivery of sludge from the discharging cone or trough. A slush or centrifugal pump subsequently removes the sludge. The thickener tanks are usually fabricated using steel sheets. But tanks with concrete sides are quite common. Some small tanks (usually < 30 m in diameter) are made of plastics. The whole assembly is installed either above ground sitting on pillars or at ground level with the discharge well below the ground level. In the latter case, an access tunnel is provided where the discharging pump is located. In some installations the discharge pump is located above the tank; in such cases, a suction pipe runs down the centre column to the bottom well. Alternatively, a submerged motor pumps the under flow slurry to the top of the tank discharging its contents to a holding tank. Several variations are known to exist. For instance the rakes are either supported by cross beams or truss above the tank or supported by the central column and cables. The cables are also connected to torque meters. Fig. 13.1 is a sketch of a bridge thickener where the bridge runs across the thickener tank. The bridge support the rakes and the motor rotating the rakes sit on a platform in the centre of the tank. The rakes are bolted to the central column which is rotated by the motor. The Bridge thickeners have a maximum diameter of about 30 meters. When the rakes are supported entirely by the central pillar, the access bridge usually runs half way on the tank surface terminating on the central pier. The centre pier thickeners are considerably larger than the Bridge type. The diameter of the tank ranges from about 35180 meters. A variation is the tray thickener where trays or compartments are placed one on top of the other. Each tray acts as a thickener and the assembly operates in parallel with a common pier or shaft where the rakes are fixed. Clarification takes place in series operation, that is, the thickener underflow from the top compartment serves as feed to the lower compartment. Ultimately the underflow from say, a six tray thickener, form the final thickened underflow. Similarly all the overflow from each tray combine forming the final overflow slurry. Fig. 13.2 is a schematic diagram of a 3compartment clarifier. Up to seven compartments are available.drive motor access bridge feed
Fig. 13.1. Sketch of a thickener showing the access bridge, feed well, rakes supported by the central column and cables and the underflow discharge.
403
overflow
feed box
Sludge Fig. 13.2 . Schematic diagram of a tray type clarifier, after Dahlstrom and Fitch [1]. The thickening process is accelerated by the addition of flocculants HiCapacity thickeners allow a mixing arrangement in the feed box where the flocculant is intimately mixed. The other design features of the HiCapacity thickeners are similar to the Bridge thickeners. While installing the feed pipe or launder to thickeners, the slope is held at 1 to 1.5. King [2] suggests that this slope provides minimum turbulence of the settling slurry in the tank. The feed is actually made to enter about a meter below the surface of the tank level thus helping to minimise turbulence. The feed well diameters are between 1 and 1.2 m with lengths of 1.2 to 5 m. Tank sizes vary according to feed characteristics and the sedimentation time. Manufacturers such as DorrOliverEimco, [3] have suggested that the water depth should be between 3.0 and 3.6 m and the feed well size about 25% of the basin area. The rakedrives in bridge clarifiers are either centre driven (as shown in the Fig. 13.1) where the motor is mounted on a support plate or are peripheral driven. When the sludge is too thick and the rakes struggle to move or in extreme cases cease altogether, the rakes are designed to rise either mechanically of pneumatically. Usually the torque on the rakes is monitored and the rakes rise automatically at a fixed torque level. This precautionary procedure is generally attached to thickeners of diameter greater than 10 meters. The allowable torque is about 530 times greater than normal operating torque [1]. A recent innovation is the DorrOliver Eimco ECat thickeners which has dispensed with the rakes and introduced clarifying cylinders through which the suspension passes to produce the clear over flow (Fig. 13.3). These thickeners are designed for rapid sedimentation by the use of flocculants. The clarified slurry then passes through filters producing a clear overflow.
404
feed overflow feed mix clarifying cylinders
cones
dewatering cones
underflow Fig. 13.3. Clarifier/Thickener, Dorr Oliver Eimco [4].
13.2. Thickener DesignBatch Process Thickeners have been designed using the basic laws of sedimentation. Empirical methods devised by manufacturers are also used for rapid work. For designing , the chief criterion is to determine the relation between the settling velocity and the dimensions of the vessel to be used for each particular slurry. The settling velocity for a particular slurry can be easily determined in the laboratory by using smallscale tests. The tests consist of determining the downward movement of the boundary of the clear liquid and the suspension. It has been found that this rate is initially constant but the rate decreased as the particles slowly settled to the bottom and the interface met the sludge zone. This can easily be visualised from Fig. 13.4 where the progressively increasing concentration with depth is shown. It is obvious that the deeper the vessel and longer the time given for settling, the clearer will be the supernatant liquid and the thicker will be the sludge. The decrease in the settling rate is due to hindrance by increased crowding of the particles as they settle and collect at the bottom of the vessel. At the sludgeforming layer, the particles pack down by displacing the liquid in between. In so doing, the clear liquid level rises. These considerations apply both to batch and continuous processes, with the difference that in the continuous process a balance between the flow rate of the overflow stream and the removal rate of the sludge has to be maintained.
405Clear fluid
time
Fig. 13.4. Sedimentation in a thickener.
These considerations originally used by Coe and Clevenger [5] are now in use extensively..The quantitative basis for designing the thickener area assumes that:
1. 2.
Settling rate was a function of concentration, The volume rate of discharge of the clear supernatant liquid was equal to the difference of the rate of feed of the slurry minus the rate of removal of the thickened layer.
For determining the thickener area, Coe and Clevenger assumed that the liquid moving upwards is always greater than the movement downwards. The mass of liquid flowing upwards is given by: t/h where F D = = = (13.1) the feed mass ratio (liquid/solids, also known as the feed dilution), discharge mass ratio (liquid/solid) and Feed capacity by mass, t/h
At equilibrium, the upward velocity of liquid equals the downward velocity of the solids. Thus if vs is the velocity of sedimentation, A the crosssectional area of the tank, in m 2 , and PL the specific gravity of the liquid, then at equilibrium: FD (13.2)
hence,
A = 
FDV
I Q M{F)
(13.3)
SPL
In practice, to determine the design value of the thickener area, a number of laboratory sedimentation tests are run using 2 litre cylinders and determining the value of vs for a range
406
of F values. The maximum value of A is taken as the design crosssectional area of the thickener tank. Dahlstrom and Fitch [2] has analysed each of the settling zones and arrived at a practical expression similar to the expression of Coe and Clevenger for sizing a thickener. Considering that the flow rate in the clear zone should be less than the settling rate of the smallest particle that has to he removed by settling, they derived the velocity of sedimentation as: vs = ^ Q (13.4)
This equation is similar to Eq. (13.2) by Coe and Clevenger. Dahlstrom and Fitch [2] suggested that the actual sedimentation rate must be multiplied by the area! efficiency factor, AEF to obtain a realistic value. The area! factor is a function of the tank dimensions (height and diameter) and ranges between 0.20 and 0.25. Eqs. (13.3) and (13.4) are extensively used to determine the crosssectional areas of tanks. The laboratory estimations are performed at different concentrations of F and D and the largest value of A is taken as the designed size of the tank as in the Coe and Clevenger method. For practical purposes they suggest a scaleup factor of 1.25  1.5 for thickener units less than 15.2 m in diameter and 1.3 1.5 for units greater than 15.2 m in diameter. 13.3. Thickener DesignContinuous Thickeners For designing continuous thickeners, the three most important parameters that need to be established are: 1. 2. 3. Cross sectional area of the tank Depth of thickened layer Depth of the clarifying zone
Other factors include discharge slurry properties, such as liquid/solid ratio, viscosity and the characteristics of pumping. 13.3.1. Estimation of CrossSectional Area of Tank Coe and Clevenger's equation fails to accurately estimate the crosssectional area of the tank when the slurry is treated with a flocculating agent. In such cases the mathematical approach of Kynch [6] as applied by Talmage and Fitch [7] is more suitable. A particular advantage is that while several determinations of settling velocities, vs, are required by Coe and Clevenger's method, a single estimation is sufficient when analysis of the sedimentation curve is made. To apply Kynch's method the following assumptions are made: 1. 2. 3. 4. The concentration of particles in any horizontal plane is uniform, Differential settling due to differences in shape, size or composition of mineral particles do not take place, The sedimentation velocity is a function of concentration and tends to zero at a concentration equivalent to the sediment layer at the bottom of the container, The wall effect is negligible.
A single laboratory test therefore involves the suspension of a slurry in a 2 litre tall transparent cylinder and measuring the clear fluid interface with the slurry at different times
407 407
till the level falls and all particles settle at the bottom as sludge. Where the sedimentation rate is very slow or the supernatant liquid remain turbid and unclear, flocculants are added. If required, rakes are introduced to break up agglomerated particles. A typical sedimentation curve indicating the height of the interface with time and the structure of the slurry in the cylinder is shown in Fig. 13.5, It can be seen that at the initial stages, the rate of fall of the interface is nearly constant. When the settling rate of the bulk of the slurry diminishes, (as seen in cylinder 4), the clear zonesludge interface merges and the curve then flattens out. At this stage, further lowering of the clear level interface can take place by the expulsion of water between the particles in the sludge. Fig.13.5 shows that at time t = 0, the height of the interface is Ho. As it is assumed that the concentration of slurry is uniform across the crosssection of the tube, at any height, Hi, the concentration of the sludge will be the same across the settling tube. For a dispersed slurry, the solids start settling at a uniform velocity which is a function of the local solids concentration [5,6]. As the settled solids build up at the bottom of the container, the boundary between the settling solids and slurry of the initial concentration starts to rise in the slurry as indicated in Fig. 13.5. Zones of intermediate concentration between the initial and final concentrations will move upwards from the bottom at a rate related to the concentration of solids in that zone. When the rising and settling zones meet, the settling slows and is controlled by the extraction of retained water from the solids as it goes through compaction. The rise velocity of the zone of concentration C, from the bottom of the cylinder to the interface of the settling mudline, vR, given by; dH dtd\j/
dC
(13.5)
and is represented by the line OY in Fig. 13.5. y is the settling flux, kg/m2/s.
Time (s)
Fig. 13.5. Settling curve Kynch's interpretation.
408
If line OY represents the initial uniform concentration Co then higher concentrations resulting from settling solids at the bottom of the cylinder are represented by lines of lower slope, OYj (for intermediate concentration) until the maximum concentration of the settled solids is reached and represented by CMAX and line OYMAX Any line parallel to these will represent the rise velocity of zones of the same concentration, C, so line H1Y1 will represent a zone of concentration Co which originates from height Hi in the slurry propagating upwards and reaching the mudline interface at Yi after time ti. Since the sedimentation rate is dependant on concentration only, until the zone of initial concentration from the cylinder bottom reaches the interface, the sedimentation rate of the interface will be constant and hence the rate vs0 will be represented by a straight line, HoY. According to Kynch, if a tangent is drawn to the settling curve at point Yt, the slope, a, corresponds to the settling velocity,vst, of the layer or zone of concentration Q just below the settling interface. The intercept of the tangent on the Yaxis, Ht, corresponds to the height of slurry of uniform concentration equal to Ct. Then by a mass balance: HtCt = H 0 C 0 (13.6)
for a cylinder of constant crosssectional area. Consequently, a plot of settling rate versus concentration can be constructed from a single settling curve. Kynch's theory has been tested experimentally on many occasions and found to hold for the batch settling of equisized rigid spheres in water but deviates for flocculated suspensions that form compressive sediments [8]. Yalcin [9] reported the sedimentation curves of a coppernickel tailings for several initial percent solids. By constructing tangents to the low density pulp curve at different higher percent solids, using the Kynch construction, estimates of the settling rates can be compared to the actual measured sedimentation rates of these slurries. Fig. 13.6 shows such a construction on the settling curve of an unflocculated slurry having an initial concentration of 5% solids. The estimates of the settling rates of the higher % solids are obtained from the tangents to the 5% sedimentation curve, intersecting the Yaxis at the mudline heights corresponding to 15, 25, 35 and 45% solids. Fig. 13.7 shows the measured sedimentation velocities versus the Kynch estimates from the slope of the tangents. The plot for the estimates from the 5% solids curve shows considerable difference from actual measured values being higher than the estimates according to the Kynch theory. If the estimates are constructed from the 15% solids curve for slurries of higher densities, Fig. 13.7 shows a closer correlation between the estimates and real sedimentation velocities. The estimates constructed from the 25% solids curve are similar to that obtained from the 15% solids curve. Figs. 13.8 and 13.9 show similar constructions for a flocculated gold tailings at 20, 30 and 40% solids. In this case, the Kynch estimates of the settling velocities are in close agreement with the actual measured velocities. Although the Kynch theory is not considered suitable for all mineral slurries, especially flocculated slurries, nevertheless it can give satisfactory results as indicated in Fig. 13.9. It is still used for thickener design calculations [8], Talmage and Fitch [7] showed that the settling velocity was related to the concentration. For a point on the settling curve of time t and height Ht, the equation is: Ct =M
H Ht+vsttt
C
(13.7)
4090.4
Ho
"35o
si
a> c
H15 H15 H25 H25H45 H450.0
I ? . A D D "0
Mudline height (m)
  55% solids % D15% 15% A25% 25%  0  335% 5% A45% 45%
A 0
40 50 60 70 80 90 100
10 10
20
30
Time (min)
Fig. 13.6. CuNi tailing sedimentation data replotted from Yalcin [9] with Kynch construction on the 5% solids curve.0.0004y y
based on 5% solids curve based on 5% curve  a  115% 5%
y
y
Kynch estimation, m/s
(A 0.0003 0.0003
  25%s*y y y
y
s'
41
n 0.0002 s . i 0.0002(A
U >
s
s
y
y
J~l
0.0001
y
,'' 0.0000 0.0000 0.0000
m 0.0001 0.0001 0.0002 0.0002
0.0003
0.0004 0.0004
measured, measured, m/s Fig. 13.7. Kynch estimated sedimentation rates compared to measured rates for different % solid slurries, (data from [9]).
4100.3
Ho
Mudline Height (m)
H1
H30H
20% solids30%40%
H40
0.0 0 0
ttTime (min)
16
Fig. 13.8. Sedimentation curves of a flocculated gold tailing with Kynch construction on the 20% solids curve.
0.0005 0.0005
Kynch estimation, m/sis
I
0.0004 0.0004
.2 0.0003 0.0003
0.0002 0.0002
0.0001 0.0001
0.0000 0.0000 0.0000 0.0000
0.0001 0.0001
0.0002 0.0002
0.0003 0.0003
0.0004 0.0004
0.0005 0.0005
measured, m/s measured, m/s
Fig. 13.9. Kynch estimated sedimentation rates compared to measured rates for a flocculated gold tailing.
411
In a batch settling test, the mass of solids in the test cylinder is given by CoHoA. If the time taken for all the solids to settle past a layer of concentration C is tu then CoHoA/tu represents the quantity of solids that can be brought through the concentration layer per unit time. The area of thickener required to settle 1 tonne of solid per unit time is then given by:A =
m2/t/h
(13.8)
The time tu is obtained by drawing a line from mudline height H, corresponding to the concentration C, at a tangent to the settling curve. The intersection of this tangent with the mudline corresponding to the underflow concentration is the value tu on the time axis. This is illustrated in Fig. 13.10. The maximum thickener area requirement will occur when the tangent is drawn through the compression point on the sedimentation curve since this tangent will give the highest value of tu in the free settling range which, according to Talmage and Fitch [6] is the zone determining the unit area. When the line, corresponding to Hu, intersects the settling curve above the compression point, the value of tu corresponding to the maximum thickener area will be the point of intersection with the settling curve, shown as tu(i) in Fig. 13.10. Fig. 13.5 shows that a near steady concentration is reached at about YMAX. Assuming this to be an equilibrium state, a material balance of solid and liquid can be made. Svarovsky [10] expressed the area of the tank in terms of the overflow rate. From a material balance, the
0.30 0.30
0.25 \ 0.25
Mudline Height (m)
g 0.20 0.20
\
I
0.15 0.15
I3
H H
V2
Critical point Critic al
HU(1) j
S 0.10 0.10

HU(2)
0.05 0.05
0.00 0.00 0
tU(1) tu(l)
4
6
8
10
12
Time (min) Time(min)
14 t U(2) 14 u ( 2 )
16 16
Fig. 13.10. Talmage and Fitch construction for determination of tu; tuOCRIT
= 0.5 x300/(0.17x60)m 2
= 14.7 m2 and diameter = 4.3 m
Considering a safety factor of 1.5, the practical diameter = 6.5 m0.18 0.18 0.16 ^ 0.16 0.14 0.14\ \
CRIT VCRIT
velocity, kg/m .s
C M
0.12 0.12 0.10 0.10 0.08 0.08 0.06 0.06 0.04 0.04 0.02 0.02 0.00 0.00 0 200 200 400 400 600 600 800 8003
2
\
\
>
\
V
/
CU Cn
/
1000 1000
1200 1200
Solids concentration, kg/m Solids concentration, kg/m
Fig. 13.22. Settling flux vs solids concentration.
In the discussions and computations explored in examples 13.1 and 13.2, the effect of different particles sizes (and possibly density) has not been considered. The velocity of descent of different sized particles will obviously be different. In such a case the sedimentation profile will consist of more than three zones (Fig. 13.23) due to the upward
429
Fig. 13.23. Sedimentation layers resulting from particles of different size and density
flow of the displaced liquid by the movement of the different size of particles. The lines of demarcation between these zones are not well defined and flux determinations are difficult. Due to such difficulties, adjustments to experimentally computed design parameters have been published from time to time to yield realistic approximations of the different parameters [1,20]. These modifications are summarised in Table 13.2. Table 13.2 Multiplying factors for different thickener parameters [20]. Parameter Tank size Sedimentation time Crosssection area of tank Transition zone depth Compression zone depth Multiplying factor 0.5  0.7 to rise rate ratio of static detention time/volume efficiency 1.2 for diameter > 30 m 1.5 for diameter < 4.6 m 1.11.25 for safety Add about 2 m 1.75
The estimated area of the tank is increased by multiplying by a factor of 1.2 for tank diameters greater than 30 meters and a factor of 1.25 for tanks with estimated diameters less than 5 meters [20]. Often the thickener area and depth are calculated by manufacturers from standard tables established from a large number of field operations. However, no two circumstances are the same and the following method adopted by Eimco [3] is of interest for rapid estimates and may be accepted with reservations. The effective clarification area is obtained from: AE = Average daily flow rate Specified overflow rate (13.38)
430 43018 18 16 16 14 14 Tank diameter, m 122
2
10 I 10
E88
C O T3
6 4 2 0 0 50 50
100 100area, Effective clarification area, m2
150 150
200 200
Fig. 13.24. Tank diameter selection [3].
where
AE = the effective clarification area = tank area  feedwell area.
The average daily flow rate is in gallons per day or m3/h and the specified overflow rate is in gallons per day per ft2 or m3/h.m2. The relation between the effective clarification area and the diameter of tank is given in Fig. 13.24. To calculate the required area for a thickener, the recommended expression is: A = Daily solid load in kilograms Floor Loading Rate (13.39)
where the solid load is in kg/day and the Floor Loading Rate is in kg/m2/day, obtained from Table 13.3. Table 13.3 Thickener floor loading [3]. % Sludge in feed 0 25 3550 75 100 Floor Loading kg/m /day 107.51 73.30 48.87 29.32 19.55 Typical % Solids in underflow 10 6 5 3 2
431
13.4. Operation of thickeners The operation of thickeners involves a delicate balance of the feed rate, the overflow rate and the underflow withdrawal rate and is dependant on the concentration of the feed, overflow and underflow streams. The feed stream generally enters the feed well at a speed of about 15 m/min but this would depend on its characteristics, such as concentration (liquid/solid ratio), particle size, particle shape and viscosity. The characteristics of the overflow and underflow streams depend on the sedimentation time and particle properties like, specific gravity, shape , size and wettability. If the particles are very small, the associated surface charge or zetapotential is of importance. Flocculants play an important role in affecting the surface charge on particles and help to accelerate or reduce the rate of sedimentation by dispersion or agglomeration. Rakes help to increase the sedimentation rate and also break up large agglomerates. The rakes are operated between 818 m/min. To prevent damage to the rakes and torque meters the recommended operation is to discharge the sludge at regular intervals at predetermined set conditions. It is necessary for the operator to detect the build up on the rakes and operate to avoid the jamming and seizure of the rakes. Usually the builtup mud tends to form islands which grows and develops a moment that could easily damage the rake mechanism. During normal operation the rise rate varies from about 0.010.03 m /min/m of crosssectional area and the detention time is between 25 hours. Some common operating parameters and crosssection of tank sizes for selected metallurgical operations are given in Table 13.4. Table 13.4. Thickener and clarifier operating conditions [1,23]. Material Copper concentrate Iron ore (concentrate, coarse) Iron ore (concentrate, fine) Lead concentrate Nickel carbonate ore (acid leach residue) Uranium (acid leach residue) Iron making blast furnace flue dust Steel making BOF flue dust Feed Underflow % solids % solids 1450 2540 1530 2025 1525 1030 0.22.0 0.22.0 4075 6075 6070 6080 4560 2565 4060 3070 Area m2/tonne/day 0.22.0 0.020.1 0.150.4 0.51.0 0.30.5 0.021.0 _ 1.53.7 1.03.7 Overflow rate m3/h/m2
13.5. Thickeners in Circuits Thickeners used to produce low solid overflows (eg. about 1% solids), may be referred to as clarifiers. Both thickeners and clarifiers are extensively used in metallurgical operations for dewatering purposes. In processing gold, nickel, iron, copper ores etc. thickeners are used to produce overflows suitable for use as process water in circuits such as flotation. The clear overflow water is used for repulping the flue dusts or fine dust from precipitators. Therefore the feed to thickeners vary considerably. A common arrangement is illustrated in Fig. 13.25
432
Feed Overflow Hydrocyclone
Sludge
Fig, 13.25. Thickener arrangement. Thickeners serve as classifiers when a near clear overflow is required. For example clarifiers used in iron blast furnace dust cleaning plant or electrostatic precipitator circuits are required to produce clean overflows as the water is for reuse and the sludge is for secondary use. In such cases the sludge is washed continuously by counter current decantation., where the underflow from a thickener/clarifier is pumped to the next thickener/clarifier (connected in series) forming the feed to the second tank. A typical set up is illustrated in Fig. 13.13 consisting of three units of thickeners/clarifiers. Such setups are structured so that the overflow from one clarifier/ thickener flows by gravity to the adjacent clarifier. The sludge is usually pumped to the next clarifier. Make up water is added at the third thickener.make up water Feed
Clarified overflow
Underflow sludge
U/F
Fig. 13.26. Thickeners in a countercurrent decantation (CCD) arrangement.
433
13.6. Problems 13.1. Settling tests in a cylindrical tube was performed on a slurry containing 300 ppm solids. After a detention time of 80 minutes, the overflow fluid was found to contain 10 ppm solids The overflow from the test data was found to be 8.2 m/h. The classifier was required to acieve an overflow rate of 120 m3/h. Estimate: 1. 2. 3. 4. The pool volume, Pool area, Pool depth, Pool diameter.
13.2. Laboratory tests on a sample of slurry showed the heights of the clear interface with time as: Height, H, mm Time, t, sec600 0 516 100 434 200 285 400 176 650 147 800 128
1000
The slurry containing 15% solids (by volume) was required to feed a continuous thickener to produce an overflow containing no more than 1% solids (by volume). Specific gravity of solids was 2.65 and water 1.0. If the feed rate is 75 t/h and the desired underflow density is 75% solids by mass, determine: 1. 2. 3. 4. The settling velocity at each time interval, The concentration of solids corresponding to each settling velocity, The fluxconcentration curve and The area of the thickener.
13.3. Using the data of problem 13.6.2, determine: 1. 2. The volume of sludge in the underflow and hence the compression zone height The height of clarification zone.
13.4. A batch settling test on a flotation tailing gave the following results. time (min)0 1 3 5 6 7
mud height (mm)340 290 236 189 175 150
time (min)8 9 10 11 15 20
mud height (mm)140 125 120 107 81 68
time (min)25 30 40 50 60
mud height (mm)63 60 58 55 55
434
Calculate the thickener area required, in m2/t/day for the following conditions.
C o = 50 kg/m3 pulp C u = 340 kg/m313.5. A settling curve of a 15% solids (by mass) copper concentrate pulp is shown in the graph below. Estimate the thickener diameter required to dewater this material to an underflow of 55 % solids (by mass) at a rate of 1000 t/h. Density of the solid is 4100 kg/m3 and water is 1000 kg/m3.
400 n 350 '
Interface Height, mm
E 300 300
H
E
J
* r 250 U)
V%A
jo 150 150
a
100
10050
t
50
0 0
J
C 0
)
10 10
20 20
30 30
40 40
50 50
60 60
70 70
1 n( m irI fir Time, min
13.6. A flocculated pulp settles according to the settling curve in the graph below. From these results, and a desired 1000 kL of clarified process water per hour from a feed slurry of 300 tph at 20% solids; 1. 2. 3. locate the critical point on the plot, What is the initial concentration of solids (Co) and the underflow concentration (Cu) in kg solid/m3 of pulp, estimate the size of thickener required using the method of Talmage and Fitch. water density = 1000 kg/m3
Data: Solids density = 2800 kg/m3
435
300
250 250
Mudline height (mm)
?200 >, 200
r"*m
jj 150 1500
c 100 = 100 O3
. a
s
50
:C 0)100 100 200 200 300 300 400 400 500 500 600 600
500
Time (s ) T im e (s)13.7 A slurry of 20% solids (by mass) is to be dewatered to produce a product of 8% moisture at 75 tph. A settling test is carried out on the slurry. The critical point of the settling curve occurs at a mudline height of 80 mm and 250 seconds. The initial mudline height in the test cylinder is 300 mm. Solid density is 2500 kg/m3 and the water density is 1000 kg/m3. 1. 2. If the mudline height corresponding to the thickener discharge is 70 mm, what would be the thickener discharge % solids? What method could be used to calculate the thickener area requirement for this slurry? Calculate the thickener diameter using this method.
13.8 A slurry of 20% solids (by mass) is to be dewatered to produce a product of 50% solids (by mass) at 75 tph (solid). A settling test is carried out on the slurry at 20%, 30% and 40% solids. The initial settling rates of the slurries are recorded below. Calculate the thickener diameter requirement for this slurry. slurry20% 30% 40%
R (mm/s) 0.7796 0.0780 0.0242
436
13.9 According to the Kyneh theory, the settling velocity of a slurry of a concentration given by the settling interface, is given by the slope of a tangent to the settling curve. If the slope to the settling curve of a flocculated copper flotation tail is 0.4 mm/s at the critical point which occurs at a point (67s, 115mm) on the settling curve, calculate the thickener area requirement to treat this slurry if the desired underflow is 65% solids (mass), the feed density is 22% solids (mass) and the initial mudline height in the settling test is 250 mm. Throughput Density of solid = 150tph = 2750 kg/m3
Density of water = 1000 kg/m3
REFERENCES [I] D.A. Dahlstrom and E.B. Fitch, in Mineral Processing Handbook, N.L. Wiess (ed), SME/AIME, Chapter 9,1985, pp. 214. [2] D.L. King, in Mineral Processing Plant Design, A.L. Mular and R.B Bhappu (eds), AIME, 1980, pp 541577. [3] Eimco 2005, Retrieved September 1,2005 from http://www.glv.com: http://www.glv.com/docs/product_docs/435/CompClarf50ft%20(pg)LR.pdf [4] Eimco 2006, Retrieved January 24,2006 from http://www.glv.com/ProductList.aspx?secID=2&catID=131 [5] H.S. Coe and G.H. Clevenger, Transactions AIMME, 55 (1916) 356. [6] GJ. Kynch, Trans. Faraday Society, 48 (1952) 166. [7] W.P. Talmage and E.B. Fitch, Industrial and Engineering Chemistry, 47 No.l (1955)38.
[8] [9] [10] [II] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21]
F. Concha and R. Burger, KONA, No. 20 (2002), 38. T. Yalcin, Bulletin of the Canadian Institute of Metallurgy, 81 No. 910 (1988) 69. L. Svarovsky, SolidLiquid Separation, Butterworths, 1977. J.J. McKetta, Unit Operations Handbook, vol.2 Mechanical Separations and Materials Handling, Marcel Dekker Inc., 1993. P. Mondal and C.B. Majumdar, Journal of the Institution of Engineers (I)  Chemical Engineering, The Institution of Engineers (India), 85 (2004) 17. E. Barnea, Chemical Engineer, (1977) 75. E.J. Roberts, Transactions, AIME, 184 (1949) 61. A. Jernqvist, Svensk Papperstidn., 68 (1965) 506, 545,578. A. Jernqvist, Svensk Papperstidn., 69 (1966) 395. E.G. Kelly and D.J. Spottiswood, Introduction to Mineral Processing, Mineral Engineering Services, Denver, 1989. N. Yoshioka, Y. Hotta, S. Tanaka, S. Naito and S. Tsugami, Chemical Engineering Japan, 21 (1957) 66. H.H. Oltmann, Filtration and Separation, 12 No. 6 (1975) 636. R.H. Perry and C.H. Chilton, Chemical Engineering Handbook, R.H. Perry and C.H. Chilton (eds), 5th Edition, McGrawHill Book Co., 1973. D.G. Osborne, SolidLiquid Separation, Chapter 5, L. Svarovsky (ed), Butterworth, London, Boston, 1977, pp. 7599.
437
[22] B. Fitch, Industrial and Engineering Chemistry, 58 (1966) 18. [23] R.H. Perry, R.H., Perry's Chemical Engineering Handbook, R.H. Perry, D.W. Green and J.O. Maloney (eds), 6th edition, Chapter 19, McGrawHill, 1984, p. 64.